Compacted oxide layer glaze describes the often shiny, wear-protective layer of oxide formed when two metals (or a metal and ceramic) are slid against each other at high temperature in an oxygen-containing atmosphere. The layer forms on either or both the surfaces in contact and can protect against wear.
Such 'glazes' have attracted limited attention due to their ability to protect the metallic surfaces on which they may form, from wear under the high temperature conditions in which they are generated. This high temperature wear protection allows potential use at temperatures beyond the range of conventional hydrocarbon-based, silicone-based or even solid lubricants such as molybdenum disulfide (the latter useful up to about 450 °C short term). Once they form, little further damage occurs unless there is a dramatic change in sliding conditions.
Such 'glazes' work by providing a mechanically resistant layer, which prevents direct contact between the two sliding surfaces. For example, when two metals slide against each other, there can be a high degree of adhesion between the surfaces. The adhesion may be sufficient to result metallic transfer from one surface to the other (or removal and ejection of such material) - effectively adhesive wear (also referred to as severe wear). With the 'glaze' layer present, such severe adhesive interactions cannot occur and wear may be greatly reduced. The continued generation of oxidized debris during the more gradual wear that results (entitled mild wear) can sustain the 'glaze' layer and maintain this low wear regime.
However, their potential application has been hampered as they have only successfully been formed under the very sliding conditions where they are meant to offer protection. A limited amount of sliding damage (referred to as 'run in wear' - actually a brief period of adhesive or severe wear) needs to occur before the oxides are generated and such 'glaze' layers can form. Efforts at encouraging their early formation have met with very limited success and the damage inflicted during the 'run in' period is one factor preventing this technique being used for practical applications.
As oxide generated is effectively the result of the tribochemical decay of one or both of the metallic (or ceramic) surfaces in contact, the study of compacted oxide layer glazes is sometimes referred to as part of the more general field of high temperature corrosion.
The generation of oxides during high temperature sliding wear does not automatically lead to the production of a compacted oxide layer 'glaze'. Under certain conditions (potentially due to incorrect conditions of sliding speed, load, temperature or oxide chemistry / composition), the oxide may not sinter together and instead the loose oxide debris may assist or enhance the removal of material by abrasive wear. A change in conditions may also see a switch from the formation of a loose, abrasive oxide to the formation of wear protective compacted oxide glaze layers and vice versa, or even the reappearance of adhesive or severe wear. Due to the complexities of the conditions controlling the types of wear observed, there have been a number of attempts to map types of wear with reference to sliding conditions in order to help better understand and predict them.
Research data from University of Port Harcourt, Department of Pharmacology update understanding of biochemistry.
Oct 19, 2010; Researchers detail in 'Antioxidants, cadmium-induced toxicity, serum biochemical and the histological abnormalities of the kidney...